Photoluminescence emission of nanoporous anodic aluminum oxide films prepared in phosphoric acid
© Nourmohammadi et al.; licensee Springer. 2012
Received: 23 October 2012
Accepted: 7 December 2012
Published: 29 December 2012
The photoluminescence emission of nanoporous anodic aluminum oxide films formed in phosphoric acid is studied in order to explore their defect-based subband electronic structure. Different excitation wavelengths are used to identify most of the details of the subband states. The films are produced under different anodizing conditions to optimize their emission in the visible range. Scanning electron microscopy investigations confirm pore formation in the produced layers. Gaussian analysis of the emission data indicates that subband states change with anodizing parameters, and various point defects can be formed both in the bulk and on the surface of these nanoporous layers during anodizing.
KeywordsAl2O3 Anodizing Phosphoric acid Oxygen vacancies Luminescence
Porous anodic aluminum oxide (PAAO) is an amorphous type of aluminum oxide, Al2O3, which is produced via anodic oxidation of aluminum in acidic electrolytes such as sulfuric, phosphoric, and oxalic acid . This nanoporous material is often used as the deposition template for fabricating one-dimensional nanostructured materials because it offers self-organized arrays of the pores in the nanoregion. The geometric coefficients of the pores such as pore size and aspect ratio can be altered over vast areas by varying the anodizing parameters. Therefore, it is possible to produce uniform one-dimensional nanomaterials with different size and aspect ratio by using these templates. Moreover, they offer the advantage of possible in situ annealing of the grown nanomaterial because of the thermal stability of aluminum oxide. PAAO films have other useful properties such as optical transparency over a wide spectral range and having low cost.
All the Al2O3 polymorphs are known as wide-band gap dielectric materials with large band gaps of 7 to 9 eV . Recently, we calculated the band gap of γ-Al2O3 compound in close agreement with experimental data . The calculations were performed in the framework of the density functional theory as embodied in the reliable WIEN2k code  using the modified Becke-Johnson (mBJ) exchange potential  by optimizing the c factor of the mBJ method. Large band gaps are assumed for different PAAO layers because the crystal structure of amorphous Al2O3 is close to the surface structure of γ-Al2O3 polymorph at room temperature . Thus, very low efficiency of free carrier photogeneration could be attributed to PAAO at room temperature. However, an interesting semiconductor behavior is observed in the barrier layer of PAAO layers which are formed in the phosphoric acid electrolyte [7–10].
As we expect, PAAO materials are insulators at room temperature, but the experimental results show that they have semiconductor behavior. This is just for existence of subband levels in the electronic structure of PAAO layers that enable carrier photogeneration at room temperature. Here, the PL properties of PAAO films formed in phosphoric acid are investigated under different anodizing conditions in order to identify the subband levels in these materials. Many detailed studies are reported in the related literature for the determination of the electronic structure of PAAO layers anodized in oxalic acid via the PL properties [11–15] because the strongest PL activity exists in these nanoporous layers. There are few articles reporting the optical properties of PAAO layers formed in different electrolytes including phosphoric acid [16, 17]. However, they have emphasized on the contribution of the type of the electrolyte, and no mention about the effect of anodizing condition on the PL properties of the anodic films formed in the phosphoric acid electrolyte. This topic is studied by us in detail.
The first part of this study is to prepare PAAO membranes through two-step anodization of high purity (99.997%, Alfa Aesar, Karlsruhe, Germany). First of all, aluminum foils are cleaned in ethanol and acetone in sequence using ultrasonic vibration, and the foil surfaces are chemically cleaned in a mixture of HCl, HNO3, and H2O with molar ratios of 10:20:70, respectively. To improve the pore order, the aluminum foils are first annealed in ambient nitrogen at 500°C to increase the aluminum grain size and reduce their internal grain boundaries in order to achieve long-range homogeneity in the foils. Then, the aluminum foil surfaces are electrochemically polished using a mixture of H3PO4, H2SO4, and H2O with 4:4:2 weight ratios, respectively . As reported in [7, 8], this process can decrease foil surface roughness down to submicron scales and remove the surface imperfections which are present on the aluminum foil after its rolling. The anodizing is carried out in a homemade anodizing cell cooled down to 2°C using high purity phosphoric acid as the electrolyte (85 wt.%, Merck, KGaA, Darmstadt, Germany). The foil temperature is kept constant at 1°C. Various anodizing voltage and time are used. After anodizing, the remaining Al substrate is etched away in a saturate solution of HgCl2 at room temperature in order to achieve transparent aluminum oxide membranes.
A VEGA- TESCAN scanning electron microscope (SEM) system (Brno, Czech Republic) is employed to confirm pore formation in the anodic layers and study size and morphology of the membrane pores. The PL spectral measurements are carried out on a PL spectroscopy LS55 system (PerkinElmer Inc., MA, USA) equipped with a Xe lamp as the light source. The PL results are Gaussian fitted, using the ‘Peak Fitter Toolbox’ in Matlab software (The MathWorks, Inc., MA, USA), in order to investigate quantitatively the effect of the anodizing parameters on the PL emissions and display formation of different point defects in the prepared membranes.
Effect of applied voltage
To evaluate the effect of anodizing voltage, both the first and the second anodizing steps are carried out by applying similar DC voltages ranging from 100 to 130 V for fix anodizing time of 20 h. This range of voltages is selected based on our previous observation on the optimized semiconductor activity of the PAAO membranes formed via aluminum anodizing at approximately 115 V for up to about 20 h .
Different excitation wavelengths are tested in order to identify most of the details of the subband states. It is observed that under 265-nm excitation wavelength, the PL emission includes most of the emission peaks which are observed by exciting the membranes under different excitation wavelengths solely. Hence, our interpretation of the defect-based subband states is based on the PL emissions measured under 265-nm excitation.
The PL emission of metal oxides usually has various origins like intrinsic electronic point defects. It is known that for isolated similar point defects in an amorphous material, the PL emission has a normal (Gaussian) shaped distribution. In the case of different light-emitting point defects, the PL emission regarding each defect type will contribute to the whole emission spectrum through a Gaussian-like peak. Gaussian fitting analyzes these contributions and assists us to identify different electronic point defects which arise in the PAAO membranes.
In Figure 3a, the 415-nm peak reveals the maximum emission intensity. This emission wavelength is close to the beginning of the blue region. However, the maximum emission locates about 427 nm in Figure 3b,c, which is close to the middle of the blue region. This wavelength shift can slightly improve the PL activity of the membranes in the visible range.
In Figure 3c, peak positions show negligible shift compared with Figure 3b. A tolerance error should be considered for both PL measurement and graph fitting procedures because the fluorescence spectrophotometer precision lies at approximately 0.1 nm, and there exists a possibility of error in the fitting process. Consequently, it could be deduced that an increase in the anodizing voltage beyond 115 V has insignificant shifting effect on the emission spectrum (see Figure 3b,c). These findings indicate that an increase in the anodizing voltage beyond 115 V cannot enhance the PL activity of the membranes in the visible range.
As a summary, it could be said that in PAAO membranes anodized in phosphoric acid, the electronic subband gaps due to oxygen vacancies can be altered by the anodizing voltage; an increase in anodizing voltage up to 115 V narrows the electronic subband gaps, and beyond 115 V, no sensible effect is observed. These results may be helpful in explaining our previous results on optimization of the room-temperature semiconductor behavior of the nanoporous layers anodized under about 115 V .
Effect of anodizing time
Different PL emissions of the samples of Figure 4 are analyzed in Figure 5 in order to evaluate the effect of anodizing time on the subband transitions quantitatively. The analyzed emission spectra of the membranes anodized at 100 V over 11- and 20-h time periods are shown in Figure 5a,b, respectively. Both spectra are composed of five contributive peaks. In Figure 5b, the same emission spectrum of Figure 3a is shown in order to compare the effect of the anodizing time on the subband transitions. The position of all Gaussian emissions of Figure 5b show a rather equal blueshift compared to the membrane of Figure 5a (see for instance peaks 1 and 2 in both figures). In Figure 5a, the maximum emission intensity takes place about 430 nm, which is close to the middle of the blue region. However, the maximum emission intensity of Figure 5b is at 415 nm which is close to the beginning of the blue region. For the membrane which is anodized for 40 h (Figure 5c), a high emission peak is observed at 394 nm which is quite close to the ultraviolet region. This confirms quantitatively widening of the electronic subband gaps due to the oxygen vacancies during a longtime anodizing process.
Some pioneering but advanced studies on PAAO layers have shown that after formation of the pores, a steady state regime of pore growth occurs . In this regime, the porous Al2O3 layer thickens with time, and no principal evolution occurs in its morphology. It might be deduced that an increase in the anodizing time would only increase the PL line intensities. However, a considerable blueshift is observed in all the PL emissions with an increase in the anodizing time (see Figure 5). This shift points out that time period of voltage application can affect the subband electronic gaps in the anodic oxide layer.
According to Huang and coworkers , F+ centers distribute mainly in the bulk structure of the PAAO layers and F centers are mainly on their surface. The anodizing electric field will drift the anions suspended in the electrolyte toward the anode (i.e., PAAO layer). Therefore, during voltage application, surface double charged oxygen vacancies can trap easily two electrons from the negatively charged anions to become neutral (F center). Our findings may confirm this argument. While the PL spectrum is gradually widened with increasing anodizing time from 11 to 40 h, the relative intensity of the first three peaks is not appreciably changed (see peaks 1 to 3 in Figure 5a,b,c). It can be deduced that these emissions originate from F+ centers which arise in the bulk of the amorphous PAAO layers during anodization in phosphoric acid.
An increase in the anodizing time from 11 to 20 h has reversed the relative intensity of the last two peaks (see peaks 4 and 5 of Figure 5a,b). Besides, the relative intensity of these two peaks is changed again after 40-h anodizing, as can be seen in Figure 5c. It can be concluded that those emissions originate from surface oxygen vacancies. Both of the mentioned emissions lay within the visible range (Figure 5). The presence of narrow band gap F centers on the surface may help us explain the semiconductor behavior of PAAO films at room temperature.
The Gaussian analysis shows that after a short anodizing time, the PL emissions are composed of five Gaussian functions (see Figure 5a,b). On the contrary, after a long anodizing, the PL spectrum has six Gaussian contributions, and an extra Gaussian emission is observed about 492 nm (within the blue-green border); see Figure 5c. This difference could be due to formation of a different-type PL emitting origin, likely an ensemble of surface oxygen vacancies, after applying voltage for a long time.
Porous anodic aluminum oxide films are successfully prepared via two-step anodization of high purity aluminum foils in phosphoric acid, and their electronic subband structure is studied via their PL emission. It is found that both the anodizing voltage and time can affect the PL emissions of the produced layers. An increase in anodizing voltage between 100 to 115 V leads to a redshift in the PL emissions and improves the PL activity of the layers in the visible region. It means that the defect-based subband gaps present in the prepared layers are narrowed. An increase in the anodizing time between 10 to 40 h shifts the PL emissions spectra toward the ultraviolet region and creates new point defects. This effect widens the defect-based subband gaps and decreases their PL activity in the visible range. Our results show that anodizing parameters that optimize the PL activity of the nanoporous layers in the visible range are close to those which optimize the semiconductor behavior of the layers at room temperature. Therefore, PL investigations could be helpful in explaining this semiconductor behavior. Most of the Al2O3 polymorphs exhibit good thermal and chemical stability and, depending on their specific properties, are used in a variety of applications. The semiconductor behavior of this type of Al2O3 makes PAAO a promising material for future applications.
Dr. AN is an assistant professor of experimental condensed matter physics at the Department of Physics, University of Isfahan, Isfahan, Iran. His research interests cover oxide and II-VI semiconductors, soft magnetic materials, and ferroelectrics. Dr. SJA is an assistant professor of computational condensed matter physics at the Department of Physics, University of Isfahan, Isfahan, Iran. Dr. SJA is interested in performing density functional theory-based ab initio calculations to study electronic, structural, hyperfine interactions including magnetic hyperfine fields and electric field gradients, quantum size effects, acoustic, and optical properties of a broad range of materials including strongly correlated systems and biomaterials in bulk, surface, interface, nanowire, and quantum dot forms. Dr. MHY is an associate professor of Nanotechnology Research Group, Faculty of Applied Sciences, Malek-Ashtar University of Technology, Shahinshahr, Isfahan, Iran. His research interests are nanomagnetism, II-VI quantum dots, and nanowires.
This work, as a part of MSc. thesis, is supported by the Office of Graduate Studies, University of Isfahan. The authors greatly appreciate Prof. M. H. Feiz and Prof. H. Sabzian from the University of Isfahan for their valuable comments, and Prof. M. Hietschold from Chemnitz University of Technology for his previous contribution.
- O’Sullivan JP, Wood GC: Morphology and mechanism of formation of porous anodic films on aluminium. P Roy Soc Lond A Mat 1970, 317: 511–543. 10.1098/rspa.1970.0129View ArticleGoogle Scholar
- Lee CK, Cho E, Lee HS, Seol KS, Han S: Comparative study of electronic structures and dielectric properties of alumina polymorphs by first-principles methods. Phys Rev B 2007, 76: 245110.View ArticleGoogle Scholar
- Yazdanmehr M, Jalali Asadabadi S, Nourmohammadi A, Ghasemzadeh M, Rezvanian M: Electronic structure and bandgap of γ-Al2O3 compound using mBJ exchange potential. Nanoscale Res Lett 2012, 7: 488. 10.1186/1556-276X-7-488View ArticleGoogle Scholar
- Blaha P, Schwarz K, Madsen GKH, Kvasnicka D, Luitz J: WIEN2k: An Augmented Plane Wave Plus Local Orbitals Program for Calculating Crystal Properties. Vienna: Vienna University of Technology; 2001.Google Scholar
- Tran F, Blaha P: Accurate band gaps of semiconductors and insulators with a semilocal exchange-correlation potential. Phys Rev Lett 2009, 102: 226401.View ArticleGoogle Scholar
- Gutiérrez G, Johansson B: Molecular dynamics study of structural properties of amorphous Al2O3. Phys Rev B 2002, 65: 104202.View ArticleGoogle Scholar
- Nourmohammadi A, Bahrevar M, Schulze S, Hietschold M: Electrodeposition of lead zirconate titanate nanotubes. J Mater Sci 2008, 43: 4753–4759. 10.1007/s10853-008-2665-3View ArticleGoogle Scholar
- Nourmohammadi A, Bahrevar MA, Hietschold M: Template-based electrophoretic deposition of perovskite PZT nanotubes. J Alloys Compd 2009, 473: 467–472. 10.1016/j.jallcom.2008.06.005View ArticleGoogle Scholar
- Nourmohammadi A, Bahrevar MA, Hietschold M: Sol–gel electrophoretic deposition of PZT nanotubes. Mater Lett 2008, 62: 3349–3351. 10.1016/j.matlet.2008.03.006View ArticleGoogle Scholar
- Nourmohammadi AH,M: Template-based electrophoretic growth of PbZrO3 nanotubes. J Sol–gel Sci Techn 2010, 53: 5.View ArticleGoogle Scholar
- Huang GS, Wu XL, Mei YF, Shao XF: Strong blue emission from anodic alumina membranes with ordered nanopore array. J Appl Phys 2003, 93: 582–585. 10.1063/1.1529075View ArticleGoogle Scholar
- Sun X, Xu F, Li Z, Zhang W: Photoluminescence properties of anodic alumina membranes with ordered nanopore arrays. J Lumin 2006, 121: 588–594. 10.1016/j.jlumin.2005.12.057View ArticleGoogle Scholar
- Du Y, Cai WL, Mo CM, Chen J, Zhang LD, Zhu XG: Preparation and photoluminescence of alumina membranes with ordered pore arrays. Appl Phys Lett 1999, 74: 2951–2953. 10.1063/1.123976View ArticleGoogle Scholar
- Stojadinovic S, Vasilic R, Nedic Z, Kasalica B, Belca I, Zekovic L: Photoluminescent properties of barrier anodic oxide films on aluminum. Thin Solid Films 2011, 519: 3516–3521. 10.1016/j.tsf.2011.01.188View ArticleGoogle Scholar
- Li Y, Li GH, Meng GW, Zhang LD, Phillipp F: Photoluminescence and optical absorption caused by the F+ centres in anodic alumina membranes. J Phys Condens Mat 2001, 13: 2691–2699. 10.1088/0953-8984/13/11/323View ArticleGoogle Scholar
- Li Z, Huang K: Blue luminescence in porous anodic alumina films. J Phys Condens Mat 2007, 19: 2163–216203.Google Scholar
- Mukhurov N, Zhvavyi S, Terekhov S, Panarin A, Kotova I, Pershukevich P, Khodasevich I, Gasenkova I, Orlovich V: Influence of electrolyte composition on photoluminescent properties of anodic aluminum oxide. J Appl Spectrosc 2008, 75: 214–218. 10.1007/s10812-008-9026-5View ArticleGoogle Scholar
- Jessensky O, Müller F, Gösele U: Self-organized formation of hexagonal pore arrays in anodic alumina. Appl Phys Lett 1998, 72: 1173–1175. 10.1063/1.121004View ArticleGoogle Scholar
- Lee KH, Crawford JH Jr: Luminescence of the F center in sapphire. Phys Rev B 1979, 19: 3217–3221. 10.1103/PhysRevB.19.3217View ArticleGoogle Scholar
- Evans BD, Pogatshnik GJ, Chen Y: Optical properties of lattice defects in α-Al2O3. Nucl Instrum Meth B 1994, 91: 258–262. 10.1016/0168-583X(94)96227-8View ArticleGoogle Scholar
- Chen W, Tang HG, Shi CS, Dang J, Shi JY, Zhou YX, Xia SD, Wang YX, Yin ST: Investigation on the origin of the blue emission in titanium doped sapphire: Is F+ color center the blue emission center? Appl Phys Lett 1995, 67: 317. 10.1063/1.115430View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.